IS 12146 (1987): Carbon manganese steel forgings for pressure … · 2018-11-15 · IS I 12146 -...
Disclosure to Promote the Right To Information Whereas the Parliament of India has set out to provide a practical regime of right to information for citizens to secure access to information under the control of public authorities, in order to promote transparency and accountability in the working of every public authority, and whereas the attached publication of the Bureau of Indian Standards is of particular interest to the public, particularly disadvantaged communities and those engaged in the pursuit of education and knowledge, the attached public safety standard is made available to promote the timely dissemination of this information in an accurate manner to the public. इंटरनेट मानक “!ान $ एक न’ भारत का +नम-ण” Satyanarayan Gangaram Pitroda “Invent a New India Using Knowledge” “प0रा1 को छोड न’ 5 तरफ” Jawaharlal Nehru “Step Out From the Old to the New” “जान1 का अ+धकार, जी1 का अ+धकार” Mazdoor Kisan Shakti Sangathan “The Right to Information, The Right to Live” “!ान एक ऐसा खजाना > जो कभी च0राया नहB जा सकता ह ै” Bhartṛhari—Nītiśatakam “Knowledge is such a treasure which cannot be stolen” IS 12146 (1987): Carbon manganese steel forgings for pressure vessels [MTD 16: Alloy Steels and Forgings]
IS 12146 (1987): Carbon manganese steel forgings for pressure … · 2018-11-15 · IS I 12146 - 1987 1. SCOPE 1.1 This standard specifies the requirements for carbon-manganese steel
Text of IS 12146 (1987): Carbon manganese steel forgings for pressure … · 2018-11-15 · IS I 12146 -...
Disclosure to Promote the Right To Information
Whereas the Parliament of India has set out to provide a practical regime of right to information for citizens to secure access to information under the control of public authorities, in order to promote transparency and accountability in the working of every public authority, and whereas the attached publication of the Bureau of Indian Standards is of particular interest to the public, particularly disadvantaged communities and those engaged in the pursuit of education and knowledge, the attached public safety standard is made available to promote the timely dissemination of this information in an accurate manner to the public.
“!ान $ एक न' भारत का +नम-ण”Satyanarayan Gangaram Pitroda
“Invent a New India Using Knowledge”
“प0रा1 को छोड न' 5 तरफ”Jawaharlal Nehru
“Step Out From the Old to the New”
“जान1 का अ+धकार, जी1 का अ+धकार”Mazdoor Kisan Shakti Sangathan
“The Right to Information, The Right to Live”
“!ान एक ऐसा खजाना > जो कभी च0राया नहB जा सकता है”Bhartṛhari—Nītiśatakam
“Knowledge is such a treasure which cannot be stolen”
“Invent a New India Using Knowledge”
IS 12146 (1987): Carbon manganese steel forgings forpressure vessels [MTD 16: Alloy Steels and Forgings]
PS : 12146 - 1987
CARBON-MANGANESE STEEL FORGINGS FOR PRESSURE VESSELS
Steel Forgings Sectional Committee, SMDC 21
DR T. MUEEERJEE
Tata Iron and Steel Go Ltd, Jamshedpur ’
SHRI S. A. HAQUE ( Alternate to Dr T. Mukherjee )
ADDITIONAL DIRECTOR ( MET ), Ministry of Railways RDSO, LUCKNOW
SHEI BRIJESH K. AWARWAL All India Metal Forging Association, New Delhi SRRI ANIL KUMAR SEARMA ( Alternate )
SHRI P. K. GAN~OPADHYAY Ministry of Defence ( DGI ) SHRI S. K. ROY ( Alternate )
SHRI R. C. JHA Steel Authority of India Ltd ( Alloy SteelPlant ), Durgapur
SHRI P. L. TALWAR ( Alternate ) SHIH V. V. KAVIS~WAH.
SRRI N. U. RAO ( Alternate ) SHRI S. S. LAEKUNDI
SHRI K. C. GO~ATE ( Alternate ) SERI S. MAZUMDAR
SHRI P. G. MULYE ( Alternate ) SHRI P. MEHRA
SHRI 0. B. DIAS ( AltErnate ) SHRI LAKSHMAN MISRA Directorate General of Technical Development,
New Delhi SARI S. V. BOPARDIKAI~ ( Alternate )
SERI H. S. RA%rAClrANDKA HMT Ltd, Bangalore SRRI P. P. C~OPRA ( Alternate I ) SHRI V. N. VENKATESAN ( Alternate II ) SHRI R. RAMPRASAD ( Alternate III ) SHRI A. SHAN~ARAM ( Alternate IV )
( Continued OR pugs 2 )
Steel Authority of India Ltd ( Bhilai Steel Plant ), Bhilai
Bharat Forge Co Ltd, Pune
Heavy Engineering Corporation, Ranchi
Association of Indian Drop Forgings and Stamping Industries, Bombay
0 Copyright 1988
BUREAU OF INDIAN STANDARDS
This publication is protected under the I&inn Copyright Act ( XIV of 1957 ) and reproduction in whole or in part by any means except with written permission of the publisher shall be deemed to be an infringement of copyright under the said Act.
( Continucdfrom page 1 )
DR B. V. REDDI Allwyn Nissan Ltd, Hyderabad SHRI J. LAKSHMIPATHI RAO ( Alternate )
Bajaj Tempo Ltd, Pune
REPRESENTATIVE Bombay Forgings Pvt Ltd, Bombay
REPRESENTATIVE Escorts Ltd, .Faridabad
REPRESENTATIVE Hindustan Motors Ltd, Uttarpara
SHRI S. SATHYANARAYANA Maruti Udyog Ltd, New Delhi Bharat Heavy Electricals Ltd, Hyderabad
SHRI ALOK SHUKLA ( Allernele I ) SHRI A. K. MITTAL ( Alternate II)
DR R. SHARAN National Institute of Foundry and Forge Techno-
DR N. M. JHA ( Alterlzate ) logy, Ranchi
SHRI S. R. SHARMA Tata Engineering and Locomotive Co Ltd,
SARI P. P. PURANIK ( Alternate ) Jamshedpur
SHRI B. B. SINGE SHRI C. K. DIXIT (Alternate )
Ministry of Defence ( DGOF )
SHRI DARBARA SINGE Directorate General of Supplies and Disposals, New Delhi
SHRI D. K. PAUL ( Alternate) SHRI SURINDER KUMAR Central Boilers Board, New Delhi Snn~ R. S. VERMA Steel Authoritv of India Ltd (Research and Deve-
DR S. MUKHERSEE ( Alternate ) lopment C&tre for Iron and Steels ), Ranchi
SH~I B. MUKHERJT, Director ( Strut & Met )
Director General, BIS ( Er-qjicio Member )
L9ecretary SHRI S. K. PANJA
Assistant Director ( Metals ), BIS
IS : 12146 - 1987
SPECIFICATION FOR CARBON-MANGANESE STEEL FORGINGS
FOR PRESSURE VESSELS
0.1 This Indian Standard was adopted by the Bureau of Indian Standards on 23 July 1987, after the draft finalized by the Steel Forgings Sectional Committee had been approved by the Structural and Metals Division Council.
0.2 This standard has been prepared to meet the need felt to have unific- ation of various grades of carbon-manganese steel forgings having low sulphur and phosphorus for use in pressure vessels and components mainly for intermediate or normal temperature service, in which weldability has also been taken into consideration.
0.3 In the preparation of this standard, assistance has been derived from the following standards:
ASTM A-434-1981 Specification for steel bars, alloy, hot-rolled or cold-finished, quenched and tempered. American Society fqr Testing and Materials.
JIS G-3202-1982 Carbon steel forgings for pressure vessels. Japanese Industrial Standards Committee.
0.4 This standard contains clauses 7.1, 9.1.2, 10.1 and 10.2 which call for agreement between the purchaser and the manufacturer.
0.5 For the purpose of deciding whether a particular requirement of this standard is complied with, the final value, observed or calculated, express- ing the result of a test or analysis, shall be rounded off in accordance with IS : 2-1960*. The number of significant places retained in the rounded off value should be the same as that of the specified value in this standard.
*Rules for rounding off numerical values ( revised ).
IS I 12146 - 1987
1.1 This standard specifies the requirements for carbon-manganese steel forgings for pressure vessels and components, mainly for intermediate or normal temperature service, in which weldability is specially taken into consideration.
2.1 For the purpose of this standard, definitions of forging terms shall be as given in IS : 1956 ( Part 6 ) - 1976*.
3. SUPPLY OF MATERIAL
3.1 General requirements relating to the supply of material shall be as laid down in IS : 1387 - 19671_.
4.1 The forgings shall be manufactured from killed steel made by only one of the primary processes like open-hearth, basic oxygen or electric furnace and may be followed by secondary steel making process.
4.2 Sufficient discard shall be made from each ingot to secure freedom from harmful piping and segregation.
4.3 Forgings shall be mechanically hot worked by a suitable process to ensure adequate deformation throughout the sections.
4.4 Heat Treatment
4.4.1 After hot working, the forgings shall be cooled so as to achieve complete transformation of austenite without any injurious effect like, cracking or distortion.
4.4.2 All forgings shall be heat-treated by annealing or normalizing, normalizing and tempering or quenching and tempering. In case of tem- pering, the temperature shall be not less than 59OOC.
4.4.3 When the purchaser desires particular heat treatment of the test piece, for example, stress relieving or any other condition, the manu- facturer shall prepare the test piece from the test specimen as specified in 9. The test piece shall be heat treated in accordance with the purchaser’s directions providing the details of the heat treatment conditions such as heat treatment temperature, soaking time, cooling rate and such other details pertinent to the specific application.
*Glossary of terms relating to iron and steel: Part 6 Forging ( including drop forg- ing ) (Jirst revision ).
tGenera1 requirements for the supply of metallurgical materials (Jirst revision ).
IS: 12146 - 1987
5. CHEMICAL COMPOSITION
5.1 Ladle Analysis - The ladle analysis of the steel when made in accordance with relevant parts of IS : 228* shall be as given in Table 1.
(1) (2) (3) (4) (5) (6) I 0’30, Max 0.35, Max 0’40 to 1’35 0’03, Max 0.03, Max II 0’35, Max 0’35, Ma.. 0.40 to 1.10 0’03, Max 0’03, Max
III 0.30, Max 0’35, Max 0.70 to 1.35 0’03, Max 0.03, Max
5.2 Product Analysis - Product analysis shall be carried out on finished forgings. The samples for product analysis shall be taken from the forging or from a full size prolongation. Samples may be taken from (1) midway between the centre and the surface of solid forgings, (2) midway between the inner and outer surfaces of hollow forgings, or (3) from broken mechanical test specimens. The chemical composition thus determined shall conform to Table 1 within the permissible variations of Table 2.
TABLE 2 PERMISSIBLE VARIATIONS IN PRODUCT ANALYSIS
ELEMENT LIMIT on MAXIMOM PERMISSIBLE VARIATION OVER THE SPECIFIED RANQE, SPECIFIED MAXIMUM LIMIT OR UNDER THE
PERCENT SPECIFIED MINIMUM LIMI’I., PERCENT Cnosa SECTIONAL AREA
T--‘--------- h______.____~ Up to and Over Over Over Over including 1 290 2 580 5 160 10 320 1290 cm8 up to up to up to cmp
2 580 5 160 10 320 cm2 cm2 cm2
includ- includ- includ- ing ing ing
(1) (2) (3) (4) (5) (6) (7) Carbon Up to and including 0.25 0.03 0’03 0’04 0’05 0’05
Over 0’25 to 0’35 inclu- 0.04 0’04 0’05 0.06 0’06 ding
Manganese Up to and including 0’90 0.04 0’05 0’06 007 0’08 Over 0’90 0’06 o-07 0.08 0’08 0’09
Silicon Up to and including 0’35 0’03 0’04 0.04 0’05 0.06 Sulphur Up to and including 0’03 0’005 0.005 0’005 0’006 0.006 Phosphorus Up to and including 0.03 0.008 0’008 0’010 0’010 0’015
NOTE: - Product cross-sectional area taken at right angles to the axis of original ingot or billet is defined as:
a) Maximum cross-sectional area of the rough machined forging excluding boring,
b\ Maximum cross-sectional area of the un-machined forging, or c) Maximum cross-sectional area of the billet, bloom or slab.
*Methods for chemical analysis of steels.
IS:12146 - 1987
6. MECHANlCAL PROPERTIES
6.1 The mechanical properties of the forgings shall be as given in Table 3.
TABLE 3 MECHANICAL PROPERTIES
GRADE TENSILETEST IHPACT TEST r--------- h --_- _--_-_ r-.-_-_-~C-_--___-~ Yield Tensile Elonga- Reduc- Test Charpy Absorbed
Strength, Strength, tion tion in Tempe- Energy (Joules ) MPa MPa Percent Area, rature *____“h_____~ (&Es) (Min) ( Min) Percent “C Mean Individual
(Min) value of value three test (A&)
(1) (2) (3) (4) (5) (6) (7) (8) I 206 412 to 550 21 38 - - -
II 245 490 to 637 18 33 - - -
III 245 490 to 637 18 38 0 27 21
7. WORKMANSHIP AND FINISH
,7.1 The forgings shall have a workman like finish and shapes, dimensions and tolerances on the forgings shall be as agreed to between the purchaser and the manufacturer.
8. FREEDOM FROM DEFECTS
8.1 The forgings shall be free from defects which affect the utility, no surface conditioning except grinding shall be permissible.
9. MECHANICAL TEST
9.1 Testing methods and types of test piece for the mechanical tests ( tensile test, IS : 1608-1972*, impact test IS : 1499-1977t, hardness test IS : 1500-1983$ ) shall be in accordance with the specification of respective standards.
9.1.1 Sampling method of specimen and number of test pieces for the forgings shall be as given in Table 4. However, when many steels are for- ged and heat treated successively at the same chance, all of them may be deemed as a single forging.
*Method for tensile testing of steel products (first revision ). tMethod for charpy impact test ( U-notch ) for metals (Jirst revision ). IMethod for Urine11 hardness test for metallic materials ( secotzd revision ).
‘IS : 12146 - 1987
Shaft shaped or cylindrical forging
TABLE 4 NUMBER OF TEST PIECES
WEIQHT OF SINQLE WEOLE LENQTIX NUMBER OF TEST FORQINQ AT TEE TIME OB HEAT
TREATING ( kg )
up to 3 000
OR HEIGHT (mm)
up to 3 000 Over 3 000
Over 3 000
- up to 1 000
One set One set each
One set each both ends
Over 1 000 Two sets at one end
up to 400 One set
Over 400 Two sets at one end
NOTE 1 - When two sets are taken from one end oflhe forging, the location of sampling of test piece shall be positioned at an angle of 180” to each other on the same side face.
NOTE 2 -When one set each is taken from both ends of the forging, the loca- tion of sampling of test piece shall be positioned at an angle of 180” to each other.
9.1.2 The specimen shall be taken from the main body of a forging or its prolongation. However, a separately forged specimen may be prepared to submit the tests when the following requirements are satisfied by agreement between the purchaser and the manufacturer:
a) The steel ingot, slab or billet made from the same molten steel as the forgings shall be used, and the same type of hot working as the forgings shall be carried out.
b) The largest forming ratio shall be not more than the smallest forming ratio of the forgings.
c) The heat treatment shall be performed at the same chance of the forging itself within the same furnace.
d) The thickness shall not be less than the largest thickness of the forgings.
9.1.3 One set of test pieces shall consist of one tensile test p~iece and further three impact test pieces when an impact test is required.
I$ : 12146 - 1987
9.1.4 Location of Sampling oj Test Piece - The location of sampling of test piece shall be as given in 188.8.131.52, 184.108.40.206 and 220.127.116.11.
18.104.22.168 For upset disc forgings and ring forgings the longitudinal axis of test specimens shall be in the tangential direction. For all other parts, the longitudinal axis of the specimens shall be parallel to the direction of major working (in case of a shaft, for example, the direction for ma.jor working is perpendicular to the axis of the shaft of the forging). When due to constraints of the geometry, it is not possible to take out specimens from specified location, for example, in case of shafts of small diameter or rings of small wall thickness, the specimens shall be taken as near the specified location as possible.
22.214.171.124 Pertaining to the forgings to be annealed, normalized, or normalized and tempered the centre of the test piece shall be located not less than l/4 T apart from the surface of a forging, where T denotes the largest thickness or diameter of the forging or separately forged specimen at the time of heat treating.
126.96.36.199 Pertaining to the forgings to be quenched and tempered, the location of sampling of test piece shall be either as given below:
a) The centte of the test piece shall be located not less than l/4 T apart from the surface of a forging and also not less than T away from the second heat treated surface. Where this method of test- ing is employed, the heat treated thickness shall generally be 75 mm, Max.
b) When the forging has so intricated shape as to be formed or machined into the similar shape of product prior to heat treat- ment, the centre of test piece shall be located apart from the heat treated surface not less than the largest distance ( t max ) be- tween the high tensile stress surface which is previously designated and the heat treated surface nearest to that surface, and as well not less than 2t max away from the second heat treated surface. However, the centre of the test piece shall be located not less than 20 mm apart from any one of heat treated surfaces and not less than 40 mm away from the second heat treated surface.
When t max is less than 20 mm, it shall be deemed as 20 mm.
c) A thermal buffer ring, at least T x T in cross section, or sections of such a ring at least 3 T in length, shall be welded to the test end of a forging prior to heat treatment for mechani- cal properties. The buffer material may be any weldable carbon or low-alloy steel which shall be joined to the forging with a par- tial penetration type weld which completely seals the buffered
IS : 12146 - 1987
surface, The test coupons shall be removed from the forging in the region buffered by the ring or ring segments. If ring segments are used, the test coupons shall be removed from the forging in the area under the centre l/3 of the buffer ring segment length. In either case, the test specimens shall be located at a minimum distance of 15 mm from the buffered surface of the forging and at least l/4 T from a quenched surface of the forging.
10.1 The manufacturer shall afford the purchaser’s inspector ~a11 reasona- ble facilities necessary to satisfy him that the material is being produced and finished in accordance with the specification. All tests and inspections shall be made at the place of manufacturer, unless otherwise agreed to between the purchaser and the manufacturer.
10.2 Repair by Welding - The defect detected through the inspection may be repaired by welding upon the agreement between the purchaser and the manufacturer.
11. ULTRASONIC TESTING
11.1 Forgings shall be ultrasonically tested to the requirements of stand- ards which may be agreed mutually between the manufacturer and the purchaser.
12.1 If the results of mechanical tests do not conform to the requirements specified, retests are permitted as outlined below:
a) If a test specimen fails to meet the minimum specified require- ments due to a flaw, other than a rupture, crack, or flake, a single retest shall be allowed.
b) In the case of failure of the mechanical test specimens to conform to the minimum requirements specified, the manufacturer may reheat-treat the forging. Testing after reheat treatment shall consist of the full number of specimens taken from locations complying with the specification or order.
c) If the average impact energy value meets specification require- ments and the energy value for one specimen is below the specifi- ed minimum value for individual specimens prescribed in Table 3, a retest is permitted of two impact specimens from a location adjacent to the specimen that has failed. Each of the retested specimens must exhibit an energy value equal to or greater than the minimum average value prescribed in Table 3.
IS : 12146 - 1987
13.1 Unless agreed otherwise, each forging shall he legibly low-stress stamped with the grade of material, heat number or identification mark and the trade mark of the manufacturer.
13.1.1 When the forgings are ordered in fully machined condition, the identification marks shall be transferred in the presence of the purchaser after full machining.
13.1.2 The forgings may also be marked’ with the Standard Mark.
NOTE - The use of the Staudard Mark is governed by the provisions of the Bureau of Indian Standards Act, 1986 and the Rules and Regulations made there- under. The Standard Mark on products covered by an Indian Standard conveys the assurance that they have been produced to comply with the requirements of that standard under a well-defitied system of inspection, testing and quality control which is devised and supervised by BIS and operated by the producer. Standard marked products are also continuously checked by BIS for conformity to that standard as a further safeguard. Details of conditions under which a licence for the use of the Standard Mark may be granted to manufacturers or producers, may be obtained from the Bureau of Indian Standards.